# Electronic Supplementary Material (ESI) for CrystEngComm.
# This journal is © The Royal Society of Chemistry 2022

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_3
_database_code_depnum_ccdc_archive 'CCDC 2061293'
loop_
_audit_author_name
_audit_author_address
'asf ziweiwie'
;Bohai University
China
;
_audit_update_record             
;
2021-11-25 deposited with the CCDC.	2021-11-29 downloaded from the CCDC.
;
_audit_creation_date             2021-11-24
_audit_creation_method           
;
Olex2 1.5
(compiled 2021.11.18 svn.ra9532c28 for OlexSys, GUI svn.r6429)
;
_shelx_SHELXL_version_number     2018/3
_chemical_name_common            ?
_chemical_name_systematic        
;
 ? 
;
_chemical_formula_moiety         'O40 Si W12, C28 H38 Co2 N12 O8, 1.5(H2 O)'
_chemical_formula_sum            'C28 H41 Co2 N12 O49.50 Si W12'
_chemical_formula_weight         3689.88
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           12
_space_group_name_H-M_alt        'C 1 2/m 1'
_space_group_name_Hall           '-C 2y'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z'
'-x, -y, -z'
'x, -y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z'

_cell_length_a                   15.8588(14)
_cell_length_b                   21.3036(14)
_cell_length_c                   10.4152(8)
_cell_angle_alpha                90
_cell_angle_beta                 98.134(2)
_cell_angle_gamma                90
_cell_volume                     3483.4(5)
_cell_formula_units_Z            2
_cell_measurement_reflns_used    2640
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      25.127
_cell_measurement_theta_min      1.628
_shelx_estimated_absorpt_T_max   0.106
_shelx_estimated_absorpt_T_min   0.085
_exptl_absorpt_coefficient_mu    20.309
_exptl_absorpt_correction_T_max  0.87
_exptl_absorpt_correction_T_min  0.86
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
;
SADABS-2016/2 (Krause et al., 2015) was used for absorption correction.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            Pink
_exptl_crystal_colour_primary    Pink
_exptl_crystal_density_diffrn    3.518
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             3290
_exptl_crystal_size_max          0.24
_exptl_crystal_size_mid          0.22
_exptl_crystal_size_min          0.2
_exptl_special_details           
;
 ? 
;
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0377
_diffrn_reflns_av_unetI/netI     0.0373
_diffrn_reflns_Laue_measured_fraction_full 0.997
_diffrn_reflns_Laue_measured_fraction_max 0.997
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_h_min       -18
_diffrn_reflns_limit_k_max       25
_diffrn_reflns_limit_k_min       -25
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       -9
_diffrn_reflns_number            10045
_diffrn_reflns_point_group_measured_fraction_full 0.997
_diffrn_reflns_point_group_measured_fraction_max 0.997
_diffrn_reflns_theta_full        25.033
_diffrn_reflns_theta_max         25.033
_diffrn_reflns_theta_min         1.611
_diffrn_ambient_temperature      296.15
_diffrn_detector                 'charge-coupled device (CCD) area detector'
_diffrn_detector_area_resol_mean 7.9
_diffrn_detector_type            'Bruker APEX II'
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device       'three-circle diffractometer'
_diffrn_measurement_device_type  'Bruker APEX II Quazar'
_diffrn_measurement_method       '0.5° ω and 0.5° φ scans'
_diffrn_radiation_collimation    'focusing mirrors'
_diffrn_radiation_detector       'Bruker APEX II'
_diffrn_radiation_monochromator  'mirror optics'
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_xray_symbol    K-L~3~
_diffrn_source                   'microfocus sealed X-ray tube'
_diffrn_source_current           30.0
_diffrn_source_power             1.2
_diffrn_source_type              'Incoatec I\ms'
_diffrn_source_voltage           40.0
_diffrn_standards_number         .
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                2529
_reflns_number_total             3158
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'SAINT+ Ver. 2016.5-0 (Bruker-AXS, 2016)'
_computing_data_collection       'APEX3 Ver. 2016.5-0 (Bruker-AXS, 2016)'
_computing_data_reduction        'SAINT+ Ver. 2016.5-0 (Bruker-AXS, 2016)'
_computing_molecular_graphics    'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2018/3 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXT 2018/2 (Sheldrick, 2018)'
_refine_diff_density_max         1.581
_refine_diff_density_min         -2.043
_refine_diff_density_rms         0.224
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.043
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     365
_refine_ls_number_reflns         3158
_refine_ls_number_restraints     73
_refine_ls_R_factor_all          0.0493
_refine_ls_R_factor_gt           0.0348
_refine_ls_restrained_S_all      1.033
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0356P)²+63.8128P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0778
_refine_ls_wR_factor_ref         0.0854
_refine_special_details          ?
_olex2_refinement_description    
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H) groups, {H1WA,H1WB} of O1W, All C(H,H) groups, All N(H) groups
 At 1.5 times of:
  All C(H,H,H) groups, {H2WA,H2WB} of O2W, {H3WA,H3WB} of O3W
2. Restrained distances
 Si1-O14
 1.535 with sigma of 0.0005
3. Uiso/Uaniso restraints and constraints
Uanis(O2W) \\sim Ueq, Uanis(O3W) \\sim Ueq: with sigma of 0.01 and sigma for
terminal atoms of 0.02
Uanis(O9) \\sim Ueq: with sigma of 0.005 and sigma for terminal atoms of 0.01
Uanis(O11) \\sim Ueq: with sigma of 0.005 and sigma for terminal atoms of 0.01
4. Rigid body (RIGU) restrains
 O1, C9, N4, O19, C5, C6, N3, C8, C2
 with sigma for 1-2 distances of 0.004 and sigma for 1-3 distances of 0.004
5. Others
 Fixed Sof: O19(0.5) O3(0.5) O6(0.5) C5(0.5) O7(0.5) C6(0.5) H6A(0.5) H6B(0.5)
 N3(0.5) O11(0.25) O13(0.25) O14(0.25) O15(0.5) O16(0.5) C8(0.5) H8A(0.5)
 H8B(0.5) O9(0.5) O4(0.5) O3A(0.5) O16A(0.5) O6A(0.5) O7A(0.5) O11A(0.25)
 O2(0.25) O2A(0.25) O2W(0.25) H2WA(0.25) H2WB(0.25) O3W(0.125) H3WA(0.125)
 H3WB(0.125) O1(0.5) C9(0.5) N4(0.5) H4(0.5)
6.a Riding coordinates:
 O1W(H1WA,H1WB), O2W(H2WA,H2WB), O3W(H3WA,H3WB)
6.b Secondary CH2 refined with riding coordinates:
 C6(H6A,H6B), C8(H8A,H8B)
6.c Me refined with riding coordinates:
 C7(H7A,H7B,H7C)
6.d Aromatic/amide H refined with riding coordinates:
 C3(H3), C1(H1), N4(H4)
;
_atom_sites_solution_hydrogens   mixed
_atom_sites_solution_primary     dual
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W 0.62354(5) 0.500000 0.30915(6) 0.04171(19) Uani 1 2 d S T P . .
Co1 Co 0.000000 0.30942(15) 0.500000 0.0737(8) Uani 1 2 d S T P . .
Si1 Si 0.500000 0.500000 0.000000 0.0220(11) Uani 1 4 d DS T P . .
C4 C 0.2504(7) 0.2632(5) 0.7183(11) 0.042(3) Uani 1 1 d . . . . .
O19 O 0.0753(14) 0.6273(11) 0.386(2) 0.050(5) Uani 0.5 1 d . . P A -1
O1W O 0.0371(7) 0.2390(7) 0.3847(14) 0.136(6) Uani 1 1 d . . . . .
H1WA H 0.083519 0.227251 0.360381 0.164 Uiso 1 1 d R U . . .
H1WB H -0.001311 0.212931 0.354681 0.164 Uiso 1 1 d R U . . .
W2 W 0.500000 0.33458(3) 0.000000 0.0480(2) Uani 1 2 d S T P . .
C3 C 0.2655(10) 0.3373(6) 0.5647(13) 0.062(4) Uani 1 1 d . . . . .
H3 H 0.300199 0.361824 0.520126 0.074 Uiso 1 1 calc R U . . .
W3 W 0.42983(3) 0.41779(2) 0.25843(4) 0.04722(17) Uani 1 1 d . . . . .
O3 O 0.6096(17) 0.3654(11) 0.074(2) 0.050(6) Uani 0.5 1 d . . P B 1
C7 C 0.2886(8) 0.2193(6) 0.8193(14) 0.060(4) Uani 1 1 d . . . . .
H7A H 0.244252 0.199512 0.858646 0.090 Uiso 1 1 calc R U . . .
H7B H 0.320577 0.187949 0.780960 0.090 Uiso 1 1 calc R U . . .
H7C H 0.325703 0.241906 0.884120 0.090 Uiso 1 1 calc R U . . .
W4 W 0.69463(3) 0.41732(3) 0.05178(5) 0.05293(18) Uani 1 1 d . . . . .
C1 C 0.1629(8) 0.2726(7) 0.6916(13) 0.056(3) Uani 1 1 d . . . . .
H1 H 0.128101 0.250991 0.741129 0.067 Uiso 1 1 calc R U . . .
O5 O 0.7861(6) 0.3775(5) 0.0776(9) 0.077(3) Uani 1 1 d . . . . .
C2 C 0.1806(11) 0.3446(7) 0.5397(14) 0.068(4) Uani 1 1 d . . . . .
O6 O 0.3276(17) 0.4006(12) 0.139(3) 0.045(6) Uani 0.5 1 d . . P B 1
C5 C 0.1507(17) 0.6162(15) 0.430(3) 0.042(6) Uani 0.5 1 d . . P A -1
O7 O 0.5362(13) 0.4376(9) 0.3613(17) 0.031(4) Uani 0.5 1 d . . P B 1
C6 C 0.1091(15) 0.4849(14) 0.307(3) 0.064(8) Uani 0.5 1 d . . P A -1
H6A H 0.082593 0.462101 0.231480 0.077 Uiso 0.5 1 calc R U P A -1
H6B H 0.064061 0.504151 0.347584 0.077 Uiso 0.5 1 calc R U P A -1
O8 O 0.6849(6) 0.500000 0.4543(11) 0.045(3) Uani 1 2 d S T P B 1
N2 N 0.3017(7) 0.2953(5) 0.6525(11) 0.057(3) Uani 1 1 d . . . . .
N1 N 0.1268(7) 0.3103(5) 0.6003(11) 0.060(3) Uani 1 1 d . . . . .
N3 N 0.1997(14) 0.5748(10) 0.376(2) 0.044(4) Uani 0.5 1 d . . P A -1
O10 O 0.500000 0.2566(6) 0.000000 0.117(8) Uani 1 2 d S T P B .
O11 O 0.7080(15) 0.500000 0.014(2) 0.036(5) Uani 0.5 2 d S TU P B 1
O12 O 0.3979(8) 0.3769(6) 0.3799(11) 0.094(4) Uani 1 1 d . . . . .
O13 O 0.4894(10) 0.500000 0.1505(16) 0.021(4) Uani 0.5 2 d S T P B .
O14 O 0.5922(4) 0.500000 0.0689(15) 0.039(5) Uani 0.5 2 d DS T P B .
O15 O 0.4575(8) 0.4382(6) 0.0416(12) 0.025(3) Uani 0.5 1 d . . P B .
O16 O 0.4708(15) 0.3384(10) 0.183(2) 0.054(6) Uani 0.5 1 d . . P B 1
C8 C 0.1633(15) 0.5352(11) 0.264(2) 0.047(5) Uani 0.5 1 d . . P A -1
H8A H 0.129543 0.561146 0.199749 0.056 Uiso 0.5 1 calc R U P A -1
H8B H 0.209070 0.516574 0.224481 0.056 Uiso 0.5 1 calc R U P A -1
O9 O 0.6533(9) 0.4388(6) 0.2005(14) 0.029(3) Uani 0.5 1 d . U P B 2
O4 O 0.7060(9) 0.4377(7) 0.2428(13) 0.032(3) Uani 0.5 1 d . . P B 1
O3A O 0.6214(15) 0.3409(10) 0.049(2) 0.042(5) Uani 0.5 1 d . . P B 2
O16A O 0.4823(12) 0.3638(8) 0.1562(18) 0.035(4) Uani 0.5 1 d . . P B 2
O6A O 0.3356(19) 0.4272(12) 0.119(3) 0.048(7) Uani 0.5 1 d . . P B 2
O7A O 0.5465(14) 0.4391(10) 0.3009(17) 0.037(5) Uani 0.5 1 d . . P B 2
O11A O 0.7612(15) 0.500000 0.050(2) 0.056(7) Uani 0.5 2 d S T P B 2
O2 O 0.405(2) 0.500000 0.267(3) 0.039(7) Uani 0.5 2 d S T P B 1
O2A O 0.389(2) 0.500000 0.321(3) 0.051(9) Uani 0.5 2 d S T P B 2
O2W O -0.019(3) 0.361(3) 0.117(6) 0.124(19) Uani 0.25 1 d . U P . .
H2WA H 0.031262 0.373176 0.115085 0.186 Uiso 0.25 1 d R U P . .
H2WB H -0.020758 0.337806 0.183735 0.186 Uiso 0.25 1 d R U P . .
O3W O -0.051(4) 0.482(3) 0.060(7) 0.07(2) Uani 0.125 1 d . U P . .
H3WA H -0.000847 0.456518 0.078551 0.100 Uiso 0.125 1 d R U P . .
H3WB H -0.089217 0.457778 0.042961 0.100 Uiso 0.125 1 d R U P . .
O1 O 0.0385(14) 0.3842(15) 0.418(3) 0.087(9) Uani 0.5 1 d . . P A -1
C9 C 0.117(2) 0.3935(18) 0.450(4) 0.059(9) Uani 0.5 1 d . . P A -1
N4 N 0.1560(13) 0.4395(11) 0.400(2) 0.051(5) Uani 0.5 1 d . . P A -1
H4 H 0.210067 0.443603 0.421734 0.061 Uiso 0.5 1 calc R U P A -1


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W1 O7 2.048(19) 6_565 ?
W1 O7 2.048(19) . ?
W1 O8 1.679(11) . ?
W1 O13 2.502(16) . ?
W1 O14 2.481(15) . ?
W1 O9 1.831(13) 6_565 ?
W1 O9 1.831(13) . ?
W1 O4 2.050(13) . ?
W1 O4 2.050(13) 6_565 ?
W1 O7A 1.78(2) . ?
W1 O7A 1.78(2) 6_565 ?
Co1 O1W 2.059(13) . ?
Co1 O1W 2.059(13) 2_556 ?
Co1 N1 2.131(11) 2_556 ?
Co1 N1 2.131(11) . ?
Co1 O1 1.95(3) . ?
Si1 O13 1.601(16) 5_665 ?
Si1 O13 1.601(16) . ?
Si1 O14 1.5351(5) 5_665 ?
Si1 O14 1.5351(5) . ?
Si1 O15 1.567(11) 5_665 ?
Si1 O15 1.567(11) . ?
Si1 O15 1.567(11) 6_565 ?
Si1 O15 1.567(11) 2_655 ?
C4 C7 1.472(17) . ?
C4 C1 1.391(17) . ?
C4 N2 1.325(14) . ?
O19 C5 1.24(3) . ?
O1W H1WA 0.8494 . ?
O1W H1WB 0.8500 . ?
W2 O3 1.92(3) 2_655 ?
W2 O3 1.92(3) . ?
W2 O10 1.661(12) . ?
W2 O15 2.366(12) 2_655 ?
W2 O15 2.366(12) . ?
W2 O16 2.03(2) . ?
W2 O16 2.03(2) 2_655 ?
W2 O3A 1.92(2) . ?
W2 O3A 1.92(2) 2_655 ?
W2 O16A 1.801(18) . ?
W2 O16A 1.801(18) 2_655 ?
C3 H3 0.9300 . ?
C3 C2 1.34(2) . ?
C3 N2 1.347(18) . ?
W3 O6 1.94(3) . ?
W3 O7 1.913(19) . ?
W3 O12 1.672(9) . ?
W3 O13 2.350(11) . ?
W3 O15 2.401(13) . ?
W3 O16 2.01(2) . ?
W3 O16A 1.844(19) . ?
W3 O6A 1.94(3) . ?
W3 O7A 1.90(2) . ?
W3 O2 1.801(7) . ?
W3 O2A 2.007(13) . ?
O3 W4 1.79(3) . ?
C7 H7A 0.9600 . ?
C7 H7B 0.9600 . ?
C7 H7C 0.9600 . ?
W4 O5 1.669(8) . ?
W4 O6 2.00(3) 2_655 ?
W4 O11 1.825(6) . ?
W4 O14 2.420(7) . ?
W4 O15 2.511(12) 2_655 ?
W4 O9 1.824(14) . ?
W4 O4 2.020(13) . ?
W4 O3A 2.00(3) . ?
W4 O6A 1.79(3) 2_655 ?
W4 O11A 2.055(12) . ?
C1 H1 0.9300 . ?
C1 N1 1.312(17) . ?
C2 N1 1.347(18) . ?
C2 C9 1.65(4) . ?
C5 N3 1.35(4) . ?
C6 H6A 0.9700 . ?
C6 H6B 0.9700 . ?
C6 C8 1.48(3) . ?
C6 N4 1.49(3) . ?
N3 C8 1.49(3) . ?
O13 O15 1.764(16) . ?
O13 O15 1.764(16) 6_565 ?
O15 O15 1.70(2) 2_655 ?
C8 H8A 0.9700 . ?
C8 H8B 0.9700 . ?
O2W H2WA 0.8500 . ?
O2W H2WB 0.8499 . ?
O3W O3W 0.78(13) 6_565 ?
O3W H3WA 0.9510 . ?
O3W H3WB 0.7966 . ?
O1 C9 1.25(4) . ?
C9 N4 1.31(4) . ?
N4 H4 0.8600 . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O7 W1 O7 81.0(11) . 6_565 ?
O7 W1 O13 68.4(6) . . ?
O7 W1 O13 68.4(6) 6_565 . ?
O7 W1 O14 102.8(5) 6_565 . ?
O7 W1 O14 102.8(5) . . ?
O7 W1 O4 99.0(7) 6_565 6_565 ?
O7 W1 O4 175.6(6) 6_565 . ?
O7 W1 O4 175.6(6) . 6_565 ?
O7 W1 O4 99.0(7) . . ?
O8 W1 O7 95.1(6) . . ?
O8 W1 O7 95.1(6) . 6_565 ?
O8 W1 O13 157.7(5) . . ?
O8 W1 O14 156.4(4) . . ?
O8 W1 O9 112.9(5) . 6_565 ?
O8 W1 O4 89.3(5) . 6_565 ?
O8 W1 O4 89.3(5) . . ?
O8 W1 O7A 110.6(6) . 6_565 ?
O14 W1 O13 45.9(4) . . ?
O9 W1 O13 82.0(5) . . ?
O9 W1 O13 82.0(5) 6_565 . ?
O9 W1 O14 53.8(4) . . ?
O9 W1 O14 53.8(4) 6_565 . ?
O9 W1 O9 90.7(8) 6_565 . ?
O4 W1 O13 107.5(5) . . ?
O4 W1 O13 107.5(5) 6_565 . ?
O4 W1 O14 72.9(4) 6_565 . ?
O4 W1 O14 72.9(4) . . ?
O4 W1 O4 80.7(8) 6_565 . ?
O7A W1 O13 56.8(7) . . ?
O7A W1 O13 56.8(7) 6_565 . ?
O7A W1 O14 85.0(6) . . ?
O7A W1 O14 85.0(6) 6_565 . ?
O7A W1 O9 136.5(7) 6_565 . ?
O7A W1 O9 71.7(8) . . ?
O7A W1 O7A 93.8(14) 6_565 . ?
O1W Co1 O1W 86.5(9) 2_556 . ?
O1W Co1 N1 88.0(4) 2_556 2_556 ?
O1W Co1 N1 92.7(4) . 2_556 ?
O1W Co1 N1 92.7(4) 2_556 . ?
O1W Co1 N1 88.0(4) . . ?
N1 Co1 N1 179.0(6) 2_556 . ?
O1 Co1 O1W 102.0(11) . . ?
O1 Co1 O1W 170.3(11) . 2_556 ?
O1 Co1 N1 96.4(8) . 2_556 ?
O1 Co1 N1 82.8(8) . . ?
O13 Si1 O13 180.0 . 5_665 ?
O14 Si1 O13 76.5(9) . . ?
O14 Si1 O13 103.5(9) . 5_665 ?
O14 Si1 O13 103.5(9) 5_665 . ?
O14 Si1 O13 76.5(9) 5_665 5_665 ?
O14 Si1 O14 180.0 . 5_665 ?
O14 Si1 O15 73.2(6) . 5_665 ?
O14 Si1 O15 73.2(6) 5_665 6_565 ?
O14 Si1 O15 106.8(6) . . ?
O14 Si1 O15 106.8(6) . 6_565 ?
O14 Si1 O15 73.2(6) 5_665 . ?
O14 Si1 O15 106.8(6) 5_665 2_655 ?
O14 Si1 O15 106.8(6) 5_665 5_665 ?
O14 Si1 O15 73.2(6) . 2_655 ?
O15 Si1 O13 67.7(5) 6_565 . ?
O15 Si1 O13 67.7(5) 5_665 5_665 ?
O15 Si1 O13 112.3(5) 2_655 . ?
O15 Si1 O13 67.7(5) . . ?
O15 Si1 O13 112.3(5) 6_565 5_665 ?
O15 Si1 O13 112.3(5) 5_665 . ?
O15 Si1 O13 67.7(5) 2_655 5_665 ?
O15 Si1 O13 112.3(5) . 5_665 ?
O15 Si1 O15 65.7(9) 5_665 6_565 ?
O15 Si1 O15 114.3(9) 5_665 2_655 ?
O15 Si1 O15 180.0(10) 6_565 2_655 ?
O15 Si1 O15 114.3(9) 6_565 . ?
O15 Si1 O15 180.0 5_665 . ?
O15 Si1 O15 65.7(9) 2_655 . ?
C1 C4 C7 122.1(11) . . ?
N2 C4 C7 118.5(11) . . ?
N2 C4 C1 119.4(12) . . ?
Co1 O1W H1WA 136.0 . . ?
Co1 O1W H1WB 116.2 . . ?
H1WA O1W H1WB 107.7 . . ?
O3 W2 O3 139.9(13) . 2_655 ?
O3 W2 O15 82.6(6) . . ?
O3 W2 O15 59.2(8) . 2_655 ?
O3 W2 O15 59.2(8) 2_655 . ?
O3 W2 O15 82.6(6) 2_655 2_655 ?
O3 W2 O16 85.5(9) 2_655 2_655 ?
O3 W2 O16 92.9(10) 2_655 . ?
O3 W2 O16 85.5(9) . . ?
O3 W2 O16 92.9(10) . 2_655 ?
O3 W2 O3A 18.7(5) 2_655 2_655 ?
O3 W2 O3A 154.1(9) . 2_655 ?
O10 W2 O3 110.0(6) . . ?
O10 W2 O3 110.0(6) . 2_655 ?
O10 W2 O15 158.9(3) . 2_655 ?
O10 W2 O15 158.9(3) . . ?
O10 W2 O16 92.3(6) . 2_655 ?
O10 W2 O16 92.3(6) . . ?
O10 W2 O3A 94.0(6) . . ?
O10 W2 O3A 94.0(6) . 2_655 ?
O10 W2 O16A 110.2(5) . 2_655 ?
O10 W2 O16A 110.2(5) . . ?
O15 W2 O15 42.1(6) 2_655 . ?
O16 W2 O15 104.1(6) 2_655 . ?
O16 W2 O15 71.5(7) . . ?
O16 W2 O15 104.1(6) . 2_655 ?
O16 W2 O15 71.5(7) 2_655 2_655 ?
O16 W2 O16 175.4(11) . 2_655 ?
O3A W2 O15 100.7(6) . . ?
O3A W2 O15 71.5(7) 2_655 . ?
O3A W2 O3A 172.0(12) 2_655 . ?
O16A W2 O15 55.1(6) . . ?
O16A W2 O15 85.9(6) 2_655 . ?
O16A W2 O3A 90.8(9) . . ?
O16A W2 O3A 86.4(10) 2_655 . ?
O16A W2 O16A 139.6(11) 2_655 . ?
C2 C3 H3 119.0 . . ?
C2 C3 N2 121.9(13) . . ?
N2 C3 H3 119.0 . . ?
O6 W3 O13 101.0(7) . . ?
O6 W3 O15 71.1(8) . . ?
O6 W3 O16 82.9(11) . . ?
O7 W3 O6 174.0(9) . . ?
O7 W3 O13 73.8(7) . . ?
O7 W3 O15 102.9(6) . . ?
O7 W3 O16 95.5(9) . . ?
O12 W3 O6 94.2(8) . . ?
O12 W3 O7 91.6(7) . . ?
O12 W3 O13 159.2(6) . . ?
O12 W3 O15 157.2(5) . . ?
O12 W3 O16 90.3(7) . . ?
O12 W3 O16A 108.8(7) . . ?
O12 W3 O6A 109.7(8) . . ?
O12 W3 O7A 109.8(7) . . ?
O12 W3 O2 112.1(10) . . ?
O12 W3 O2A 93.6(9) . . ?
O13 W3 O15 43.6(4) . . ?
O16 W3 O13 105.5(6) . . ?
O16 W3 O15 71.0(6) . . ?
O16A W3 O13 86.8(6) . . ?
O16A W3 O15 54.0(6) . . ?
O16A W3 O6A 89.7(12) . . ?
O16A W3 O7A 77.2(8) . . ?
O16A W3 O2A 157.5(9) . . ?
O6A W3 O13 83.3(7) . . ?
O6A W3 O15 60.1(9) . . ?
O6A W3 O2A 84.3(15) . . ?
O7A W3 O13 59.2(7) . . ?
O7A W3 O15 82.7(6) . . ?
O7A W3 O6A 140.6(8) . . ?
O7A W3 O2A 93.7(12) . . ?
O2 W3 O6 92.6(15) . . ?
O2 W3 O7 86.6(13) . . ?
O2 W3 O13 53.5(9) . . ?
O2 W3 O15 86.6(10) . . ?
O2 W3 O16 157.4(10) . . ?
O2A W3 O13 71.0(7) . . ?
O2A W3 O15 104.8(9) . . ?
W4 O3 W2 145.0(14) . . ?
C4 C7 H7A 109.5 . . ?
C4 C7 H7B 109.5 . . ?
C4 C7 H7C 109.5 . . ?
H7A C7 H7B 109.5 . . ?
H7A C7 H7C 109.5 . . ?
H7B C7 H7C 109.5 . . ?
O3 W4 O6 89.3(12) . 2_655 ?
O3 W4 O11 137.7(10) . . ?
O3 W4 O14 85.1(7) . . ?
O3 W4 O15 57.2(8) . 2_655 ?
O3 W4 O4 88.2(8) . . ?
O3 W4 O6A 95.8(13) . 2_655 ?
O5 W4 O3 108.6(8) . . ?
O5 W4 O6 95.5(7) . 2_655 ?
O5 W4 O11 113.6(8) . . ?
O5 W4 O14 159.3(4) . . ?
O5 W4 O15 156.7(5) . 2_655 ?
O5 W4 O9 113.6(5) . . ?
O5 W4 O4 89.8(5) . . ?
O5 W4 O3A 94.5(7) . . ?
O5 W4 O6A 109.0(8) . 2_655 ?
O5 W4 O11A 90.0(7) . . ?
O6 W4 O14 100.2(7) 2_655 . ?
O6 W4 O15 67.8(7) 2_655 2_655 ?
O6 W4 O4 174.6(8) 2_655 . ?
O11 W4 O6 88.0(11) . 2_655 ?
O11 W4 O14 54.1(7) . . ?
O11 W4 O15 83.0(8) . 2_655 ?
O11 W4 O4 90.6(8) . . ?
O14 W4 O15 44.0(3) . 2_655 ?
O9 W4 O14 55.1(6) . . ?
O9 W4 O3A 86.5(7) . . ?
O9 W4 O11A 92.2(8) . . ?
O4 W4 O14 74.8(5) . . ?
O4 W4 O15 106.9(5) . 2_655 ?
O3A W4 O14 101.5(6) . . ?
O3A W4 O11A 175.4(8) . . ?
O6A W4 O14 84.2(7) 2_655 . ?
O6A W4 O9 137.5(8) 2_655 . ?
O6A W4 O3A 90.4(13) 2_655 . ?
O6A W4 O11A 87.5(12) 2_655 . ?
O11A W4 O14 74.2(6) . . ?
C4 C1 H1 118.2 . . ?
N1 C1 C4 123.7(12) . . ?
N1 C1 H1 118.2 . . ?
C3 C2 N1 122.0(14) . . ?
C3 C2 C9 134.6(17) . . ?
N1 C2 C9 103.2(16) . . ?
W3 O6 W4 128.3(12) . 2_655 ?
O19 C5 N3 124(3) . . ?
W3 O7 W1 124.8(10) . . ?
H6A C6 H6B 107.6 . . ?
C8 C6 H6A 108.7 . . ?
C8 C6 H6B 108.7 . . ?
C8 C6 N4 114.2(18) . . ?
N4 C6 H6A 108.7 . . ?
N4 C6 H6B 108.7 . . ?
C4 N2 C3 117.3(12) . . ?
C1 N1 Co1 129.4(9) . . ?
C1 N1 C2 115.5(12) . . ?
C2 N1 Co1 113.1(10) . . ?
C5 N3 C8 121(2) . . ?
W4 O11 W4 149.7(13) 6_565 . ?
Si1 O13 W1 116.7(8) . . ?
Si1 O13 W3 125.0(5) . . ?
Si1 O13 W3 125.0(5) . 6_565 ?
Si1 O13 O15 55.2(6) . . ?
Si1 O13 O15 55.2(6) . 6_565 ?
W3 O13 W1 92.6(5) . . ?
W3 O13 W1 92.6(5) 6_565 . ?
W3 O13 W3 96.4(6) 6_565 . ?
O15 O13 W1 124.3(7) 6_565 . ?
O15 O13 W1 124.3(7) . . ?
O15 O13 W3 140.0(10) . 6_565 ?
O15 O13 W3 140.0(10) 6_565 . ?
O15 O13 W3 69.8(5) . . ?
O15 O13 W3 69.8(5) 6_565 6_565 ?
O15 O13 O15 96.5(11) . 6_565 ?
Si1 O14 W1 120.9(9) . . ?
Si1 O14 W4 124.8(4) . 6_565 ?
Si1 O14 W4 124.8(4) . . ?
W4 O14 W1 91.9(2) . . ?
W4 O14 W1 91.9(2) 6_565 . ?
W4 O14 W4 93.4(3) . 6_565 ?
Si1 O15 W2 126.1(7) . . ?
Si1 O15 W3 123.7(6) . . ?
Si1 O15 W4 118.0(7) . 2_655 ?
Si1 O15 O13 57.1(6) . . ?
Si1 O15 O15 57.1(5) . 2_655 ?
W2 O15 W3 95.6(4) . . ?
W2 O15 W4 92.7(4) . 2_655 ?
W3 O15 W4 92.2(4) . 2_655 ?
O13 O15 W2 138.7(8) . . ?
O13 O15 W3 66.7(6) . . ?
O13 O15 W4 123.6(8) . 2_655 ?
O15 O15 W2 68.9(3) 2_655 . ?
O15 O15 W3 137.9(10) 2_655 . ?
O15 O15 W4 126.1(10) 2_655 2_655 ?
O15 O15 O13 98.8(9) 2_655 . ?
W3 O16 W2 122.0(9) . . ?
C6 C8 N3 110(2) . . ?
C6 C8 H8A 109.6 . . ?
C6 C8 H8B 109.6 . . ?
N3 C8 H8A 109.6 . . ?
N3 C8 H8B 109.6 . . ?
H8A C8 H8B 108.1 . . ?
W4 O9 W1 149.2(8) . . ?
W4 O4 W1 119.9(7) . . ?
W2 O3A W4 128.2(10) . . ?
W2 O16A W3 151.4(12) . . ?
W4 O6A W3 143(2) 2_655 . ?
W1 O7A W3 146.0(12) . . ?
W4 O11A W4 118.0(11) 6_565 . ?
W3 O2 W3 153.1(19) 6_565 . ?
W3 O2A W3 121.5(13) 6_565 . ?
H2WA O2W H2WB 109.5 . . ?
O3W O3W H3WA 124.3 6_565 . ?
O3W O3W H3WB 129.7 6_565 . ?
H3WA O3W H3WB 105.9 . . ?
C9 O1 Co1 112(2) . . ?
O1 C9 C2 124(3) . . ?
O1 C9 N4 122(3) . . ?
N4 C9 C2 114(3) . . ?
C6 N4 H4 119.2 . . ?
C9 N4 C6 122(2) . . ?
C9 N4 H4 119.2 . . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
W1 O13 O15 Si1 -100.8(10) . . . . ?
W1 O13 O15 W2 8.2(17) . . . . ?
W1 O13 O15 W3 78.9(7) . . . . ?
W1 O13 O15 W4 155.2(6) . . . 2_655 ?
W1 O13 O15 O15 -59.8(11) . . . 2_655 ?
Co1 O1 C9 C2 5(4) . . . . ?
Co1 O1 C9 N4 176(3) . . . . ?
Si1 O13 O15 W2 109.0(11) . . . . ?
Si1 O13 O15 W3 179.8(7) . . . . ?
Si1 O13 O15 W4 -103.9(9) . . . 2_655 ?
Si1 O13 O15 O15 41.0(7) . . . 2_655 ?
C4 C1 N1 Co1 156.7(10) . . . . ?
C4 C1 N1 C2 -5.8(19) . . . . ?
O19 C5 N3 C8 -5(4) . . . . ?
W2 O3 W4 O5 -129.8(17) . . . . ?
W2 O3 W4 O6 -34.2(19) . . . 2_655 ?
W2 O3 W4 O11 52(2) . . . . ?
W2 O3 W4 O14 66.2(18) . . . . ?
W2 O3 W4 O15 29.6(15) . . . 2_655 ?
W2 O3 W4 O4 141.1(18) . . . . ?
C3 C2 N1 Co1 -160.7(11) . . . . ?
C3 C2 N1 C1 5(2) . . . . ?
C3 C2 C9 O1 164(3) . . . . ?
C3 C2 C9 N4 -8(5) . . . . ?
W3 O13 O15 Si1 105.0(11) 6_565 . . . ?
W3 O13 O15 Si1 -179.8(7) . . . . ?
W3 O13 O15 W2 -146.0(8) 6_565 . . . ?
W3 O13 O15 W2 -70.7(11) . . . . ?
W3 O13 O15 W3 -75.2(12) 6_565 . . . ?
W3 O13 O15 W4 76.3(7) . . . 2_655 ?
W3 O13 O15 W4 1.1(17) 6_565 . . 2_655 ?
W3 O13 O15 O15 -138.7(8) . . . 2_655 ?
W3 O13 O15 O15 146.1(11) 6_565 . . 2_655 ?
O3 W4 O11 W4 58(3) . . . 6_565 ?
C7 C4 C1 N1 -178.4(12) . . . . ?
C7 C4 N2 C3 -177.1(11) . . . . ?
C1 C4 N2 C3 2.0(17) . . . . ?
O5 W4 O11 W4 -120(3) . . . 6_565 ?
O5 W4 O9 W1 117.0(17) . . . . ?
C2 C3 N2 C4 -3.0(19) . . . . ?
C2 C9 N4 C6 175(2) . . . . ?
O6 W3 O2 W3 -129(5) . . . 6_565 ?
O6 W4 O11 W4 144(3) 2_655 . . 6_565 ?
C5 N3 C8 C6 -74(3) . . . . ?
O7 W3 O2 W3 45(5) . . . 6_565 ?
N2 C4 C1 N1 2.6(19) . . . . ?
N2 C3 C2 N1 0(2) . . . . ?
N2 C3 C2 C9 174(2) . . . . ?
N1 C2 C9 O1 -20(4) . . . . ?
N1 C2 C9 N4 168(3) . . . . ?
O10 W2 O16A W3 -135.6(19) . . . . ?
O12 W3 O16A W2 136(2) . . . . ?
O12 W3 O7A W1 -130.7(18) . . . . ?
O12 W3 O2 W3 136(4) . . . 6_565 ?
O13 W1 O9 W4 82.4(17) . . . . ?
O13 W1 O7A W3 -28.6(15) . . . . ?
O13 Si1 O14 W1 180.000(0) 5_665 . . . ?
O13 Si1 O14 W1 0.000(0) . . . . ?
O13 Si1 O14 W4 -117.6(9) . . . 6_565 ?
O13 Si1 O14 W4 117.6(9) . . . . ?
O13 Si1 O14 W4 -62.4(9) 5_665 . . . ?
O13 Si1 O14 W4 62.4(9) 5_665 . . 6_565 ?
O13 Si1 O15 W2 -129.4(10) . . . . ?
O13 Si1 O15 W2 50.6(10) 5_665 . . . ?
O13 Si1 O15 W3 179.7(7) 5_665 . . . ?
O13 Si1 O15 W3 -0.3(7) . . . . ?
O13 Si1 O15 W4 -66.3(9) 5_665 . . 2_655 ?
O13 Si1 O15 W4 113.7(9) . . . 2_655 ?
O13 Si1 O15 O13 179.999(3) 5_665 . . . ?
O13 Si1 O15 O15 50.6(10) 5_665 . . 2_655 ?
O13 Si1 O15 O15 -129.4(10) . . . 2_655 ?
O13 W3 O16A W2 -58(2) . . . . ?
O13 W3 O7A W1 29.8(16) . . . . ?
O13 W3 O2 W3 -27(4) . . . 6_565 ?
O14 W1 O9 W4 42.6(15) . . . . ?
O14 W1 O7A W3 -67.5(18) . . . . ?
O14 Si1 O13 W1 180.000(0) 5_665 . . . ?
O14 Si1 O13 W1 0.000(0) . . . . ?
O14 Si1 O13 W3 114.5(8) . . . 6_565 ?
O14 Si1 O13 W3 -65.5(8) 5_665 . . 6_565 ?
O14 Si1 O13 W3 65.5(8) 5_665 . . . ?
O14 Si1 O13 W3 -114.5(8) . . . . ?
O14 Si1 O13 O15 65.2(5) 5_665 . . . ?
O14 Si1 O13 O15 114.8(5) . . . 6_565 ?
O14 Si1 O13 O15 -114.8(5) . . . . ?
O14 Si1 O13 O15 -65.2(5) 5_665 . . 6_565 ?
O14 Si1 O15 W2 -62.2(10) . . . . ?
O14 Si1 O15 W2 117.8(10) 5_665 . . . ?
O14 Si1 O15 W3 -113.0(10) 5_665 . . . ?
O14 Si1 O15 W3 67.0(10) . . . . ?
O14 Si1 O15 W4 1.0(7) 5_665 . . 2_655 ?
O14 Si1 O15 W4 -179.0(7) . . . 2_655 ?
O14 Si1 O15 O13 67.3(9) . . . . ?
O14 Si1 O15 O13 -112.7(9) 5_665 . . . ?
O14 Si1 O15 O15 117.8(10) 5_665 . . 2_655 ?
O14 Si1 O15 O15 -62.2(10) . . . 2_655 ?
O14 W4 O11 W4 40(2) . . . 6_565 ?
O14 W4 O9 W1 -43.0(15) . . . . ?
O15 Si1 O13 W1 -114.8(5) 6_565 . . . ?
O15 Si1 O13 W1 65.2(5) 2_655 . . . ?
O15 Si1 O13 W1 -65.2(5) 5_665 . . . ?
O15 Si1 O13 W1 114.8(5) . . . . ?
O15 Si1 O13 W3 -0.3(8) 6_565 . . 6_565 ?
O15 Si1 O13 W3 179.7(8) 2_655 . . 6_565 ?
O15 Si1 O13 W3 49.3(11) 5_665 . . 6_565 ?
O15 Si1 O13 W3 -49.3(11) 2_655 . . . ?
O15 Si1 O13 W3 0.3(7) . . . . ?
O15 Si1 O13 W3 130.7(11) 6_565 . . . ?
O15 Si1 O13 W3 -130.7(11) . . . 6_565 ?
O15 Si1 O13 W3 -179.7(7) 5_665 . . . ?
O15 Si1 O13 O15 -49.6(11) 2_655 . . . ?
O15 Si1 O13 O15 -130.4(11) . . . 6_565 ?
O15 Si1 O13 O15 179.999(3) 5_665 . . . ?
O15 Si1 O13 O15 130.4(11) 6_565 . . . ?
O15 Si1 O13 O15 180.000(4) 2_655 . . 6_565 ?
O15 Si1 O13 O15 49.6(11) 5_665 . . 6_565 ?
O15 Si1 O14 W1 -61.3(5) . . . . ?
O15 Si1 O14 W1 118.7(5) 5_665 . . . ?
O15 Si1 O14 W1 -118.7(5) 2_655 . . . ?
O15 Si1 O14 W1 61.3(5) 6_565 . . . ?
O15 Si1 O14 W4 -56.3(12) 6_565 . . 6_565 ?
O15 Si1 O14 W4 1.1(8) 5_665 . . 6_565 ?
O15 Si1 O14 W4 56.3(12) . . . . ?
O15 Si1 O14 W4 -178.9(8) . . . 6_565 ?
O15 Si1 O14 W4 178.9(8) 6_565 . . . ?
O15 Si1 O14 W4 -1.1(8) 2_655 . . . ?
O15 Si1 O14 W4 -123.7(12) 5_665 . . . ?
O15 Si1 O14 W4 123.7(12) 2_655 . . 6_565 ?
O15 Si1 O15 W2 0.000(2) 2_655 . . . ?
O15 Si1 O15 W2 180.000(1) 6_565 . . . ?
O15 Si1 O15 W3 129.1(12) 2_655 . . . ?
O15 Si1 O15 W3 -50.9(12) 6_565 . . . ?
O15 Si1 O15 W4 -116.9(11) 2_655 . . 2_655 ?
O15 Si1 O15 W4 63.1(11) 6_565 . . 2_655 ?
O15 Si1 O15 O13 129.4(10) 2_655 . . . ?
O15 Si1 O15 O13 -50.6(10) 6_565 . . . ?
O15 Si1 O15 O15 180.000(1) 6_565 . . 2_655 ?
O15 W2 O16A W3 27.3(18) . . . . ?
O15 W2 O16A W3 58(2) 2_655 . . . ?
O15 W3 O16A W2 -27.3(18) . . . . ?
O15 W3 O7A W1 69.0(18) . . . . ?
O15 W3 O2 W3 -58(5) . . . 6_565 ?
O15 W4 O11 W4 77(3) 2_655 . . 6_565 ?
O15 W4 O9 W1 -82.1(17) 2_655 . . . ?
O15 O13 O15 Si1 39.0(8) 6_565 . . . ?
O15 O13 O15 W2 148.0(6) 6_565 . . . ?
O15 O13 O15 W3 -141.2(9) 6_565 . . . ?
O15 O13 O15 W4 -64.9(12) 6_565 . . 2_655 ?
O15 O13 O15 O15 80.1(11) 6_565 . . 2_655 ?
O16 W3 O2 W3 -51(7) . . . 6_565 ?
C8 C6 N4 C9 178(3) . . . . ?
O9 W1 O9 W4 1(2) 6_565 . . . ?
O9 W1 O7A W3 -121(2) . . . . ?
O9 W1 O7A W3 -50(2) 6_565 . . . ?
O4 W4 O11 W4 -30(3) . . . 6_565 ?
O3A W2 O16A W3 130(2) . . . . ?
O3A W2 O16A W3 -43(2) 2_655 . . . ?
O3A W4 O9 W1 -149.6(18) . . . . ?
O16A W2 O16A W3 44.4(19) 2_655 . . . ?
O16A W3 O7A W1 124(2) . . . . ?
O6A W3 O16A W2 25(2) . . . . ?
O6A W3 O7A W1 50(3) . . . . ?
O6A W4 O9 W1 -63(3) 2_655 . . . ?
O7A W1 O9 W4 140.0(19) . . . . ?
O7A W1 O9 W4 64(2) 6_565 . . . ?
O7A W1 O7A W3 17(2) 6_565 . . . ?
O7A W3 O16A W2 -118(2) . . . . ?
O11A W4 O9 W1 26.0(18) . . . . ?
O2A W3 O16A W2 -49(5) . . . . ?
O2A W3 O7A W1 -35(2) . . . . ?
O1 C9 N4 C6 3(5) . . . . ?
C9 C2 N1 Co1 23.0(19) . . . . ?
C9 C2 N1 C1 -171.5(18) . . . . ?
N4 C6 C8 N3 -63(3) . . . . ?

_platon_squeeze_special_details  ?
_olex2_submission_special_instructions 'No special instructions were received'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_4
_database_code_depnum_ccdc_archive 'CCDC 2061294'
loop_
_audit_author_name
_audit_author_address
'asf ziweiwie'
;Bohai University
China
;
_audit_update_record             
;
2021-11-25 deposited with the CCDC.	2021-11-29 downloaded from the CCDC.
;
_audit_creation_date             2021-11-20
_audit_creation_method           
;
Olex2 1.5
(compiled 2021.11.18 svn.ra9532c28 for OlexSys, GUI svn.r6427)
;
_shelx_SHELXL_version_number     2018/3
_chemical_name_common            ?
_chemical_name_systematic        
;
 ? 
;
_chemical_formula_moiety         'C28 H32 Cu2 N12 O44 Si W12, 8(H2 O)'
_chemical_formula_sum            'C28 H48 Cu2 N12 O52 Si W12'
_chemical_formula_weight         3746.15
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        'P 1 21/n 1'
_space_group_name_Hall           '-P 2yn'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, -y-1/2, z-1/2'

_cell_length_a                   10.1453(7)
_cell_length_b                   17.1380(11)
_cell_length_c                   19.2588(12)
_cell_angle_alpha                90
_cell_angle_beta                 96.218(2)
_cell_angle_gamma                90
_cell_volume                     3328.8(4)
_cell_formula_units_Z            2
_cell_measurement_reflns_used    1283
_cell_measurement_temperature    273(2)
_cell_measurement_theta_max      21.88
_cell_measurement_theta_min      2.34
_shelx_estimated_absorpt_T_max   ?
_shelx_estimated_absorpt_T_min   ?
_exptl_absorpt_coefficient_mu    21.398
_exptl_absorpt_correction_T_max  0.87
_exptl_absorpt_correction_T_min  0.86
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
;
SADABS-2016/2 (Krause et al., 2015) was used for absorption correction.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            blue
_exptl_crystal_colour_primary    blue
_exptl_crystal_density_diffrn    3.737
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             3352
_exptl_crystal_size_max          0.24
_exptl_crystal_size_mid          0.22
_exptl_crystal_size_min          0.2
_exptl_special_details           
;
 ? 
;
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.1145
_diffrn_reflns_av_unetI/netI     0.1232
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.999
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       19
_diffrn_reflns_limit_k_min       -20
_diffrn_reflns_limit_l_max       13
_diffrn_reflns_limit_l_min       -23
_diffrn_reflns_number            19979
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.999
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         25.696
_diffrn_reflns_theta_min         1.595
_diffrn_ambient_temperature      273.15
_diffrn_detector                 'charge-coupled device (CCD) area detector'
_diffrn_detector_area_resol_mean 7.9
_diffrn_detector_type            'Bruker APEX II'
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device       'three-circle diffractometer'
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_collimation    'focusing mirrors'
_diffrn_radiation_detector       'Bruker APEX II'
_diffrn_radiation_monochromator  'mirror optics'
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_xray_symbol    K-L~3~
_diffrn_source                   'microfocus sealed X-ray tube'
_diffrn_source_current           30.0
_diffrn_source_power             1.2
_diffrn_source_type              'Incoatec I\ms'
_diffrn_source_voltage           40.0
_diffrn_standards_number         0
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                3916
_reflns_number_total             6339
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'SAINT V8.18C (?, 2016)'
_computing_data_collection       'APEX3 Ver. 2016.5-0 (Bruker-AXS, 2016)'
_computing_data_reduction        'SAINT V8.18C (?, 2016)'
_computing_molecular_graphics    'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2018/3 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXT 2018/2 (Sheldrick, 2018)'
_refine_diff_density_max         1.868
_refine_diff_density_min         -2.327
_refine_diff_density_rms         0.380
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.075
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     574
_refine_ls_number_reflns         6339
_refine_ls_number_restraints     744
_refine_ls_R_factor_all          0.1286
_refine_ls_R_factor_gt           0.0689
_refine_ls_restrained_S_all      1.021
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+115.4300P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1058
_refine_ls_wR_factor_ref         0.1225
_refine_special_details          ?
_olex2_refinement_description    
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H) groups, All C(H,H) groups, All N(H) groups
 At 1.5 times of:
  All C(H,H,H) groups, All O(H,H) groups
2. Uiso/Uaniso restraints and constraints
Uanis(O15) \\sim Ueq, Uanis(O15A) \\sim Ueq, Uanis(O18A) \\sim Ueq, Uanis(O18)
\\sim Ueq, Uanis(O5) \\sim Ueq, Uanis(O12) \\sim Ueq, Uanis(O16) \\sim Ueq,
Uanis(O10A) \\sim Ueq, Uanis(O21) \\sim Ueq, Uanis(O10) \\sim Ueq: with sigma
of 0.01 and sigma for terminal atoms of 0.02
3. Rigid body (RIGU) restrains
 All non-hydrogen atoms
 with sigma for 1-2 distances of 0.004 and sigma for 1-3 distances of 0.004
4. Others
 Fixed Sof: O5(0.5) O5A(0.5) O10(0.5) O10A(0.5) O11(0.5) O11A(0.5) O12(0.5)
 O12A(0.5) O14(0.5) O14A(0.5) O15(0.5) O15A(0.5) O16(0.5) O16A(0.5) O18(0.5)
 O18A(0.5) O21(0.5) O22(0.5) O23(0.5) O24(0.5)
5.a Riding coordinates:
 O1W(H1WA,H1WB), O2W(H2WA,H2WB), O3W(H3WA,H3WB), O4W(H4WA,H4WB)
5.b Secondary CH2 refined with riding coordinates:
 C13(H13A,H13B), C14(H14A,H14B)
5.c Me refined with riding coordinates:
 C7(H7A,H7B,H7C), C12(H12A,H12B,H12C)
5.d Aromatic/amide H refined with riding coordinates:
 N3(H3), N4(H4), C2(H2), C3(H3A), C8(H8), C9(H9)
;
_atom_sites_solution_hydrogens   mixed
_atom_sites_solution_primary     dual
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W -0.02038(10) 0.43638(6) 0.32634(5) 0.0294(3) Uani 1 1 d . . . . .
W2 W 0.20437(10) 0.66122(6) 0.55490(5) 0.0366(3) Uani 1 1 d . . . . .
W3 W 0.27930(10) 0.41340(6) 0.43495(6) 0.0390(3) Uani 1 1 d . . . . .
W4 W 0.17510(10) 0.60120(7) 0.37978(5) 0.0395(3) Uani 1 1 d . . . . .
W5 W -0.09661(13) 0.68960(6) 0.44871(6) 0.0470(3) Uani 1 1 d . . . . .
W6 W 0.29642(10) 0.47042(6) 0.61128(5) 0.0330(3) Uani 1 1 d . . . . .
Cu1 Cu 0.3466(3) 0.75814(17) 0.26876(14) 0.0304(7) Uani 1 1 d . . . . .
Si1 Si 0.000000 0.500000 0.500000 0.024(2) Uani 1 2 d S . P . .
O1 O 0.4508(14) 0.7809(8) 0.3577(7) 0.027(3) Uani 1 1 d . . . . .
O2 O 0.7399(14) 0.7723(8) 0.6828(8) 0.029(4) Uani 1 1 d . . . . .
O3 O 0.2613(15) 0.6485(8) 0.3215(8) 0.033(3) Uani 1 1 d . . . . .
O4 O 0.1050(17) 0.6454(10) 0.6329(9) 0.049(4) Uani 1 1 d . . . . .
O5 O 0.304(3) 0.5098(18) 0.3861(16) 0.026(5) Uani 0.5 1 d . U P A 1
O5A O 0.279(3) 0.5209(17) 0.4196(15) 0.022(5) Uani 0.5 1 d . . P A 2
O6 O 0.1760(17) 0.5041(10) 0.6754(9) 0.047(4) Uani 1 1 d . . . . .
O7 O -0.1457(16) 0.7801(9) 0.4238(9) 0.045(4) Uani 1 1 d . . . . .
O8 O 0.3035(17) 0.7380(9) 0.5808(9) 0.051(4) Uani 1 1 d . . . . .
O9 O 0.216(2) 0.3733(10) 0.6118(9) 0.063(5) Uani 1 1 d . . . . .
O10 O -0.234(3) 0.6769(18) 0.5147(17) 0.026(7) Uani 0.5 1 d . U P A 1
O10A O -0.165(3) 0.6682(17) 0.5249(16) 0.023(6) Uani 0.5 1 d . U P A 2
O11 O 0.046(3) 0.6892(18) 0.3804(15) 0.027(6) Uani 0.5 1 d . . P A 1
O11A O 0.012(3) 0.642(2) 0.3855(17) 0.032(6) Uani 0.5 1 d . . P A 2
O12 O 0.079(3) 0.5303(18) 0.3016(17) 0.029(5) Uani 0.5 1 d . U P A 1
O12A O 0.058(3) 0.5393(19) 0.3385(17) 0.031(5) Uani 0.5 1 d . . P A 2
O13 O 0.4056(15) 0.3712(10) 0.4049(10) 0.054(5) Uani 1 1 d . . . . .
O14 O 0.063(3) 0.7333(17) 0.5147(16) 0.027(5) Uani 0.5 1 d . . P A 1
O14A O 0.034(3) 0.6887(18) 0.5224(18) 0.034(5) Uani 0.5 1 d . . P A 2
O15 O 0.150(3) 0.3867(18) 0.3441(17) 0.028(6) Uani 0.5 1 d . U P A 1
O15A O 0.131(3) 0.4025(18) 0.3781(17) 0.028(5) Uani 0.5 1 d . U P A 2
O16 O 0.275(3) 0.6679(17) 0.4594(16) 0.027(5) Uani 0.5 1 d . U P A 1
O16A O 0.228(3) 0.6242(18) 0.4676(16) 0.030(5) Uani 0.5 1 d . . P A 2
O17 O -0.032(2) 0.4069(11) 0.2428(9) 0.064(5) Uani 1 1 d . . . . .
O18 O 0.393(3) 0.4396(18) 0.5320(17) 0.034(5) Uani 0.5 1 d . U P A 1
O18A O 0.319(3) 0.4553(17) 0.5185(16) 0.028(5) Uani 0.5 1 d . U P A 2
O19 O 0.3104(15) 0.5776(9) 0.5874(9) 0.042(3) Uani 1 1 d . . . . .
O20 O 0.4303(16) 0.4564(13) 0.6677(9) 0.068(6) Uani 1 1 d . . . . .
O21 O -0.076(3) 0.5148(15) 0.5729(14) 0.020(5) Uani 0.5 1 d . U P A .
O22 O 0.060(3) 0.5912(15) 0.4800(15) 0.023(4) Uani 0.5 1 d . . P A .
O23 O -0.084(3) 0.4680(16) 0.4382(16) 0.030(5) Uani 0.5 1 d . . P A .
O24 O 0.138(3) 0.4440(16) 0.5239(16) 0.029(4) Uani 0.5 1 d . . P A .
N1 N 0.9915(18) 0.7895(10) 0.7239(9) 0.026(4) Uani 1 1 d . . . . .
N2 N 0.2101(18) 0.8203(10) 0.3076(9) 0.027(4) Uani 1 1 d . . . . .
N3 N 0.4381(16) 0.8356(10) 0.4624(8) 0.024(4) Uani 1 1 d . . . . .
H3 H 0.391864 0.861442 0.489373 0.029 Uiso 1 1 calc R U . . .
N4 N 0.7449(18) 0.8387(10) 0.5827(10) 0.034(4) Uani 1 1 d . . . . .
H4 H 0.790987 0.864075 0.555264 0.041 Uiso 1 1 calc R U . . .
N5 N 0.0375(19) 0.8987(11) 0.3852(10) 0.034(4) Uani 1 1 d . . . . .
N6 N 1.1628(19) 0.8697(11) 0.6499(10) 0.033(4) Uani 1 1 d . . . . .
C1 C 0.804(2) 0.8114(12) 0.6413(12) 0.026(4) Uani 1 1 d . . . . .
C2 C 1.115(2) 0.7943(13) 0.7468(12) 0.030(5) Uani 1 1 d . . . . .
H2 H 1.145574 0.771529 0.789368 0.036 Uiso 1 1 calc R U . . .
C3 C 1.036(2) 0.8649(14) 0.6254(13) 0.036(6) Uani 1 1 d . . . . .
H3A H 1.006863 0.890348 0.583977 0.043 Uiso 1 1 calc R U . . .
C4 C 0.384(2) 0.8190(12) 0.4003(11) 0.024(5) Uani 1 1 d . . . . .
C5 C 0.246(2) 0.8408(13) 0.3744(11) 0.026(5) Uani 1 1 d . . . . .
C6 C 0.946(2) 0.8233(11) 0.6594(10) 0.019(4) Uani 1 1 d . . . . .
C7 C 1.352(2) 0.8338(15) 0.7284(12) 0.043(6) Uani 1 1 d . . . . .
H7A H 1.373079 0.806100 0.771508 0.064 Uiso 1 1 calc R U . . .
H7B H 1.394928 0.809014 0.692204 0.064 Uiso 1 1 calc R U . . .
H7C H 1.382176 0.886732 0.733884 0.064 Uiso 1 1 calc R U . . .
C8 C 0.164(2) 0.8828(13) 0.4121(12) 0.035(6) Uani 1 1 d . . . . .
H8 H 0.195148 0.900514 0.456558 0.042 Uiso 1 1 calc R U . . .
C9 C 0.091(2) 0.8387(14) 0.2801(13) 0.042(6) Uani 1 1 d . . . . .
H9 H 0.066216 0.826324 0.233594 0.050 Uiso 1 1 calc R U . . .
C10 C 1.202(2) 0.8330(15) 0.7087(12) 0.037(5) Uani 1 1 d . . . . .
C11 C 0.001(2) 0.8764(14) 0.3179(12) 0.035(5) Uani 1 1 d . . . . .
C12 C -0.138(2) 0.8964(16) 0.2856(12) 0.052(8) Uani 1 1 d . . . . .
H12A H -0.150320 0.877413 0.238452 0.078 Uiso 1 1 calc R U . . .
H12B H -0.201590 0.872407 0.312242 0.078 Uiso 1 1 calc R U . . .
H12C H -0.149602 0.951962 0.285662 0.078 Uiso 1 1 calc R U . . .
C13 C 0.570(2) 0.8137(17) 0.4893(12) 0.046(7) Uani 1 1 d . . . . .
H13A H 0.631971 0.841569 0.463099 0.056 Uiso 1 1 calc R U . . .
H13B H 0.581388 0.758478 0.480713 0.056 Uiso 1 1 calc R U . . .
C14 C 0.607(2) 0.8282(17) 0.5624(12) 0.051(7) Uani 1 1 d . . . . .
H14A H 0.560452 0.874483 0.575568 0.062 Uiso 1 1 calc R U . . .
H14B H 0.576238 0.784741 0.588701 0.062 Uiso 1 1 calc R U . . .
O1W O 0.8632(19) 0.9446(10) 0.4903(8) 0.057(5) Uani 1 1 d . . . . .
H1WA H 0.803576 0.977168 0.484895 0.086 Uiso 1 1 d R U . . .
H1WB H 0.901536 0.938408 0.453685 0.086 Uiso 1 1 d R U . . .
O2W O 0.3255(16) 0.9443(10) 0.5600(8) 0.050(5) Uani 1 1 d . . . . .
H2WA H 0.299657 0.915268 0.591858 0.075 Uiso 1 1 d R U . . .
H2WB H 0.388007 0.976008 0.572598 0.075 Uiso 1 1 d R U . . .
O3W O 0.441(3) 0.9969(13) 0.3645(12) 0.108(9) Uani 1 1 d . . . . .
H3WA H 0.439541 0.967066 0.330765 0.163 Uiso 1 1 d R U . . .
H3WB H 0.364631 1.015146 0.364735 0.163 Uiso 1 1 d R U . . .
O4W O 0.318(2) 0.5212(14) 0.2221(12) 0.101(8) Uani 1 1 d . . . . .
H4WA H 0.404191 0.516455 0.227588 0.151 Uiso 1 1 d R U . . .
H4WB H 0.302081 0.557255 0.250398 0.151 Uiso 1 1 d R U . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W1 O4 1.861(16) 3_566 ?
W1 O6 1.877(17) 3_566 ?
W1 O12 1.99(3) . ?
W1 O12A 1.94(3) . ?
W1 O15 1.93(3) . ?
W1 O15A 1.83(3) . ?
W1 O17 1.677(17) . ?
W1 O21 2.24(3) 3_566 ?
W1 O23 2.38(3) . ?
W2 O4 1.918(15) . ?
W2 O8 1.697(16) . ?
W2 O14 1.98(3) . ?
W2 O14A 1.84(3) . ?
W2 O16 2.05(3) . ?
W2 O16A 1.84(3) . ?
W2 O19 1.859(16) . ?
W2 O22 2.28(3) . ?
W3 O5 1.93(3) . ?
W3 O5A 1.87(3) . ?
W3 O10 1.91(3) 3_566 ?
W3 O10A 2.03(3) 3_566 ?
W3 O13 1.632(15) . ?
W3 O15 2.12(3) . ?
W3 O15A 1.77(3) . ?
W3 O18 2.13(3) . ?
W3 O18A 1.77(3) . ?
W3 O21 2.39(3) 3_566 ?
W3 O24 2.41(3) . ?
W4 O3 1.702(14) . ?
W4 O5 2.03(3) . ?
W4 O5A 1.85(3) . ?
W4 O11 2.00(3) . ?
W4 O11A 1.81(3) . ?
W4 O12 2.09(3) . ?
W4 O12A 1.72(3) . ?
W4 O16 2.09(3) . ?
W4 O16A 1.76(3) . ?
W4 O21 2.45(2) 3_566 ?
W4 O22 2.37(3) . ?
W5 O7 1.682(15) . ?
W5 O9 1.922(19) 3_566 ?
W5 O10 2.00(3) . ?
W5 O10A 1.73(3) . ?
W5 O11 2.06(3) . ?
W5 O11A 1.91(3) . ?
W5 O14 2.09(3) . ?
W5 O14A 1.83(3) . ?
W5 O22 2.35(3) . ?
W5 O24 2.40(3) 3_566 ?
W6 O6 1.917(16) . ?
W6 O9 1.852(17) . ?
W6 O18 1.97(3) . ?
W6 O18A 1.84(3) . ?
W6 O19 1.903(15) . ?
W6 O20 1.662(17) . ?
W6 O23 2.49(3) 3_566 ?
W6 O24 2.24(3) . ?
Cu1 O1 1.952(14) . ?
Cu1 O2 1.948(14) 4_575 ?
Cu1 O3 2.345(14) . ?
Cu1 N1 1.962(18) 4_575 ?
Cu1 N2 1.958(18) . ?
Si1 O21 1.69(3) . ?
Si1 O21 1.69(3) 3_566 ?
Si1 O22 1.73(3) . ?
Si1 O22 1.73(3) 3_566 ?
Si1 O23 1.49(3) 3_566 ?
Si1 O23 1.49(3) . ?
Si1 O24 1.72(3) . ?
Si1 O24 1.72(3) 3_566 ?
O1 C4 1.30(2) . ?
O2 C1 1.28(2) . ?
O21 O23 1.69(4) 3_566 ?
O23 O24 1.79(4) 3_566 ?
N1 C2 1.28(3) . ?
N1 C6 1.40(2) . ?
N2 C5 1.35(3) . ?
N2 C9 1.30(3) . ?
N3 H3 0.8600 . ?
N3 C4 1.29(2) . ?
N3 C13 1.43(3) . ?
N4 H4 0.8600 . ?
N4 C1 1.31(3) . ?
N4 C14 1.42(3) . ?
N5 C8 1.36(3) . ?
N5 C11 1.36(3) . ?
N6 C3 1.32(3) . ?
N6 C10 1.32(3) . ?
C1 C6 1.46(3) . ?
C2 H2 0.9300 . ?
C2 C10 1.38(3) . ?
C3 H3A 0.9300 . ?
C3 C6 1.38(3) . ?
C4 C5 1.48(3) . ?
C5 C8 1.37(3) . ?
C7 H7A 0.9600 . ?
C7 H7B 0.9600 . ?
C7 H7C 0.9600 . ?
C7 C10 1.53(3) . ?
C8 H8 0.9300 . ?
C9 H9 0.9300 . ?
C9 C11 1.39(3) . ?
C11 C12 1.52(3) . ?
C12 H12A 0.9600 . ?
C12 H12B 0.9600 . ?
C12 H12C 0.9600 . ?
C13 H13A 0.9700 . ?
C13 H13B 0.9700 . ?
C13 C14 1.44(3) . ?
C14 H14A 0.9700 . ?
C14 H14B 0.9700 . ?
O1W H1WA 0.8215 . ?
O1W H1WB 0.8480 . ?
O2W H2WA 0.8537 . ?
O2W H2WB 0.8502 . ?
O3W H3WA 0.8254 . ?
O3W H3WB 0.8401 . ?
O4W H4WA 0.8766 . ?
O4W H4WB 0.8497 . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O4 W1 O6 89.5(7) 3_566 3_566 ?
O4 W1 O12 169.0(11) 3_566 . ?
O4 W1 O12A 146.8(11) 3_566 . ?
O4 W1 O15 92.2(11) 3_566 . ?
O4 W1 O21 95.5(8) 3_566 3_566 ?
O4 W1 O23 66.9(8) 3_566 . ?
O6 W1 O12 90.3(11) 3_566 . ?
O6 W1 O12A 80.9(11) 3_566 . ?
O6 W1 O15 168.9(11) 3_566 . ?
O6 W1 O21 95.8(9) 3_566 3_566 ?
O6 W1 O23 65.3(9) 3_566 . ?
O12 W1 O21 73.6(11) . 3_566 ?
O12 W1 O23 103.2(12) . . ?
O12A W1 O23 80.3(11) . . ?
O15 W1 O12 85.9(13) . . ?
O15 W1 O21 73.1(11) . 3_566 ?
O15 W1 O23 105.5(12) . . ?
O15A W1 O12A 85.0(14) . . ?
O15A W1 O23 82.7(12) . . ?
O17 W1 O4 100.8(9) . 3_566 ?
O17 W1 O6 100.0(8) . 3_566 ?
O17 W1 O12 90.0(12) . . ?
O17 W1 O12A 112.1(12) . . ?
O17 W1 O15 90.5(11) . . ?
O17 W1 O15A 113.3(12) . . ?
O17 W1 O21 157.3(10) . 3_566 ?
O17 W1 O23 159.8(10) . . ?
O21 W1 O23 42.8(9) 3_566 . ?
O4 W2 O14 88.6(9) . . ?
O4 W2 O16 167.6(10) . . ?
O4 W2 O22 93.7(9) . . ?
O8 W2 O4 103.0(8) . . ?
O8 W2 O14 90.7(11) . . ?
O8 W2 O14A 114.1(12) . . ?
O8 W2 O16 88.0(10) . . ?
O8 W2 O16A 113.9(11) . . ?
O8 W2 O19 101.3(8) . . ?
O8 W2 O22 155.8(9) . . ?
O14 W2 O16 85.6(11) . . ?
O14 W2 O22 72.2(11) . . ?
O14A W2 O4 75.4(12) . . ?
O14A W2 O16A 89.3(14) . . ?
O14A W2 O19 143.3(11) . . ?
O14A W2 O22 53.2(12) . . ?
O16 W2 O22 74.2(11) . . ?
O16A W2 O4 143.2(11) . . ?
O16A W2 O19 85.1(11) . . ?
O16A W2 O22 51.6(11) . . ?
O19 W2 O4 87.8(7) . . ?
O19 W2 O14 168.0(10) . . ?
O19 W2 O16 95.7(10) . . ?
O19 W2 O22 96.7(8) . . ?
O5 W3 O10A 152.5(13) . 3_566 ?
O5 W3 O15 83.3(13) . . ?
O5 W3 O18 99.2(13) . . ?
O5 W3 O21 71.6(11) . 3_566 ?
O5 W3 O24 106.2(11) . . ?
O5A W3 O24 84.7(11) . . ?
O10 W3 O5 173.0(13) 3_566 . ?
O10 W3 O10A 21.1(10) 3_566 3_566 ?
O10 W3 O15 94.8(13) 3_566 . ?
O10 W3 O18 82.0(13) 3_566 . ?
O10 W3 O21 101.4(11) 3_566 3_566 ?
O10 W3 O24 67.7(11) 3_566 . ?
O10A W3 O24 57.8(10) 3_566 . ?
O13 W3 O5 93.4(11) . . ?
O13 W3 O5A 111.6(11) . . ?
O13 W3 O10 93.5(11) . 3_566 ?
O13 W3 O10A 109.6(11) . 3_566 ?
O13 W3 O15 92.8(11) . . ?
O13 W3 O15A 112.3(12) . . ?
O13 W3 O18 91.9(11) . . ?
O13 W3 O18A 113.2(12) . . ?
O13 W3 O21 155.6(9) . 3_566 ?
O13 W3 O24 154.2(10) . . ?
O15 W3 O18 174.4(12) . . ?
O15 W3 O21 66.9(10) . 3_566 ?
O15 W3 O24 105.8(11) . . ?
O15A W3 O5A 91.2(14) . . ?
O15A W3 O24 86.1(13) . . ?
O18 W3 O21 109.1(11) . 3_566 ?
O18 W3 O24 68.8(11) . . ?
O18A W3 O5A 74.9(13) . . ?
O18A W3 O15A 134.3(15) . . ?
O18A W3 O24 50.0(12) . . ?
O21 W3 O24 50.0(9) 3_566 . ?
O3 W4 O5 91.9(10) . . ?
O3 W4 O5A 108.5(10) . . ?
O3 W4 O11 91.6(10) . . ?
O3 W4 O11A 113.2(11) . . ?
O3 W4 O12 91.9(10) . . ?
O3 W4 O12A 111.5(11) . . ?
O3 W4 O16 88.8(9) . . ?
O3 W4 O16A 113.7(11) . . ?
O3 W4 O21 153.3(8) . 3_566 ?
O3 W4 O22 155.0(8) . . ?
O5 W4 O12 80.8(12) . . ?
O5 W4 O16 96.8(12) . . ?
O5 W4 O21 68.8(11) . 3_566 ?
O5 W4 O22 105.4(11) . . ?
O5A W4 O22 85.4(11) . . ?
O11 W4 O5 176.0(12) . . ?
O11 W4 O12 101.0(13) . . ?
O11 W4 O16 81.3(12) . . ?
O11 W4 O21 108.5(11) . 3_566 ?
O11 W4 O22 70.6(11) . . ?
O11A W4 O5A 138.4(13) . . ?
O11A W4 O22 56.2(12) . . ?
O12 W4 O21 67.6(11) . 3_566 ?
O12 W4 O22 108.2(11) . . ?
O12A W4 O5A 93.9(14) . . ?
O12A W4 O11A 71.3(15) . . ?
O12A W4 O16A 134.8(14) . . ?
O12A W4 O22 87.4(12) . . ?
O16 W4 O12 177.6(12) . . ?
O16 W4 O21 111.0(10) . 3_566 ?
O16 W4 O22 71.7(10) . . ?
O16A W4 O5A 70.6(13) . . ?
O16A W4 O11A 92.3(14) . . ?
O16A W4 O22 50.3(12) . . ?
O22 W4 O21 51.6(9) . 3_566 ?
O7 W5 O9 101.3(8) . 3_566 ?
O7 W5 O10 94.3(10) . . ?
O7 W5 O10A 107.7(11) . . ?
O7 W5 O11 91.6(10) . . ?
O7 W5 O11A 112.6(11) . . ?
O7 W5 O14 91.7(10) . . ?
O7 W5 O14A 113.3(12) . . ?
O7 W5 O22 155.0(8) . . ?
O7 W5 O24 152.8(9) . 3_566 ?
O9 W5 O10 83.4(11) 3_566 . ?
O9 W5 O11 93.1(10) 3_566 . ?
O9 W5 O14 165.7(10) 3_566 . ?
O9 W5 O22 96.8(9) 3_566 . ?
O9 W5 O24 58.9(9) 3_566 3_566 ?
O10 W5 O11 173.6(12) . . ?
O10 W5 O14 101.7(12) . . ?
O10 W5 O22 104.9(11) . . ?
O10 W5 O24 66.8(11) . 3_566 ?
O10A W5 O11A 139.7(14) . . ?
O10A W5 O14A 70.2(15) . . ?
O10A W5 O22 87.1(12) . . ?
O11 W5 O14 80.5(11) . . ?
O11 W5 O22 70.0(11) . . ?
O11 W5 O24 106.8(11) . 3_566 ?
O11A W5 O22 55.8(12) . . ?
O14 W5 O22 69.1(11) . . ?
O14 W5 O24 110.6(11) . 3_566 ?
O14A W5 O11A 94.1(14) . . ?
O14A W5 O22 52.0(12) . . ?
O22 W5 O24 52.2(9) . 3_566 ?
O6 W6 O18 169.4(11) . . ?
O6 W6 O23 62.2(9) . 3_566 ?
O6 W6 O24 95.1(9) . . ?
O9 W6 O6 87.5(7) . . ?
O9 W6 O18 91.0(10) . . ?
O9 W6 O19 155.9(8) . . ?
O9 W6 O23 91.2(9) . 3_566 ?
O9 W6 O24 62.9(9) . . ?
O18 W6 O23 107.3(12) . 3_566 ?
O18 W6 O24 75.0(12) . . ?
O18A W6 O6 145.1(11) . . ?
O18A W6 O9 88.8(11) . . ?
O18A W6 O19 83.2(10) . . ?
O18A W6 O24 53.0(12) . . ?
O19 W6 O6 86.2(7) . . ?
O19 W6 O18 90.9(10) . . ?
O19 W6 O23 65.4(8) . 3_566 ?
O19 W6 O24 94.6(9) . . ?
O20 W6 O6 99.0(8) . . ?
O20 W6 O9 101.2(10) . . ?
O20 W6 O18 91.6(12) . . ?
O20 W6 O18A 115.8(12) . . ?
O20 W6 O19 102.8(9) . . ?
O20 W6 O23 157.2(10) . 3_566 ?
O20 W6 O24 158.3(10) . . ?
O24 W6 O23 43.9(9) . 3_566 ?
O1 Cu1 O3 88.3(6) . . ?
O1 Cu1 N1 96.3(7) . 4_575 ?
O1 Cu1 N2 84.0(7) . . ?
O2 Cu1 O1 175.6(6) 4_575 . ?
O2 Cu1 O3 87.5(6) 4_575 . ?
O2 Cu1 N1 83.6(7) 4_575 4_575 ?
O2 Cu1 N2 96.8(7) 4_575 . ?
N1 Cu1 O3 100.7(6) 4_575 . ?
N2 Cu1 O3 87.8(7) . . ?
N2 Cu1 N1 171.5(7) . 4_575 ?
O21 Si1 O21 180.0 . 3_566 ?
O21 Si1 O22 75.5(12) 3_566 . ?
O21 Si1 O22 104.5(12) . . ?
O21 Si1 O22 75.5(12) . 3_566 ?
O21 Si1 O22 104.5(12) 3_566 3_566 ?
O21 Si1 O24 107.1(13) . . ?
O21 Si1 O24 72.9(13) . 3_566 ?
O21 Si1 O24 107.1(13) 3_566 3_566 ?
O21 Si1 O24 72.9(13) 3_566 . ?
O22 Si1 O22 180.0(18) 3_566 . ?
O23 Si1 O21 116.3(13) 3_566 3_566 ?
O23 Si1 O21 116.3(13) . . ?
O23 Si1 O21 63.7(13) 3_566 . ?
O23 Si1 O21 63.7(13) . 3_566 ?
O23 Si1 O22 109.7(14) 3_566 3_566 ?
O23 Si1 O22 109.7(14) . . ?
O23 Si1 O22 70.3(14) . 3_566 ?
O23 Si1 O22 70.3(14) 3_566 . ?
O23 Si1 O23 180.0 3_566 . ?
O23 Si1 O24 112.8(15) . . ?
O23 Si1 O24 67.2(15) 3_566 . ?
O23 Si1 O24 112.8(15) 3_566 3_566 ?
O23 Si1 O24 67.2(15) . 3_566 ?
O24 Si1 O22 105.7(13) . . ?
O24 Si1 O22 74.3(13) . 3_566 ?
O24 Si1 O22 74.3(13) 3_566 . ?
O24 Si1 O22 105.7(13) 3_566 3_566 ?
O24 Si1 O24 180.0 . 3_566 ?
C4 O1 Cu1 112.6(13) . . ?
C1 O2 Cu1 113.5(14) . 4_676 ?
W4 O3 Cu1 155.2(9) . . ?
W1 O4 W2 137.9(10) 3_566 . ?
W3 O5 W4 124.9(15) . . ?
W4 O5A W3 142.2(18) . . ?
W1 O6 W6 138.2(10) 3_566 . ?
W6 O9 W5 138.5(10) . 3_566 ?
W3 O10 W5 129.3(16) 3_566 . ?
W5 O10A W3 140.3(17) . 3_566 ?
W4 O11 W5 120.9(15) . . ?
W4 O11A W5 142.9(19) . . ?
W1 O12 W4 120.5(15) . . ?
W4 O12A W1 150.5(19) . . ?
W2 O14 W5 119.6(14) . . ?
W5 O14A W2 147.3(19) . . ?
W1 O15 W3 121.0(15) . . ?
W3 O15A W1 155(2) . . ?
W2 O16 W4 116.0(13) . . ?
W4 O16A W2 154.0(18) . . ?
W6 O18 W3 117.9(16) . . ?
W3 O18A W6 154.1(18) . . ?
W2 O19 W6 140.3(9) . . ?
W1 O21 W3 99.0(10) 3_566 3_566 ?
W1 O21 W4 98.0(10) 3_566 3_566 ?
W3 O21 W4 93.3(8) 3_566 3_566 ?
Si1 O21 W1 125.2(13) . 3_566 ?
Si1 O21 W3 119.6(13) . 3_566 ?
Si1 O21 W4 115.5(13) . 3_566 ?
O23 O21 W1 72.9(14) 3_566 3_566 ?
O23 O21 W3 137.5(17) 3_566 3_566 ?
O23 O21 W4 128.9(17) 3_566 3_566 ?
O23 O21 Si1 52.3(13) 3_566 . ?
W2 O22 W4 97.8(9) . . ?
W2 O22 W5 98.9(10) . . ?
W5 O22 W4 96.8(10) . . ?
Si1 O22 W2 123.3(14) . . ?
Si1 O22 W4 117.5(13) . . ?
Si1 O22 W5 117.5(13) . . ?
W1 O23 W6 93.3(11) . 3_566 ?
Si1 O23 W1 128.3(16) . . ?
Si1 O23 W6 123.0(16) . 3_566 ?
Si1 O23 O21 64.0(14) . 3_566 ?
Si1 O23 O24 62.5(14) . 3_566 ?
O21 O23 W1 64.3(13) 3_566 . ?
O21 O23 W6 133.0(17) 3_566 3_566 ?
O21 O23 O24 104.2(19) 3_566 3_566 ?
O24 O23 W1 133.4(18) 3_566 . ?
O24 O23 W6 60.6(13) 3_566 3_566 ?
W5 O24 W3 94.6(9) 3_566 . ?
W6 O24 W3 98.3(11) . . ?
W6 O24 W5 99.0(11) . 3_566 ?
Si1 O24 W3 117.4(15) . . ?
Si1 O24 W5 115.9(14) . 3_566 ?
Si1 O24 W6 125.8(15) . . ?
Si1 O24 O23 50.3(13) . 3_566 ?
O23 O24 W3 134.9(17) 3_566 . ?
O23 O24 W5 130.4(17) 3_566 3_566 ?
O23 O24 W6 75.5(15) 3_566 . ?
C2 N1 Cu1 128.6(16) . 4_676 ?
C2 N1 C6 119(2) . . ?
C6 N1 Cu1 112.0(14) . 4_676 ?
C5 N2 Cu1 112.0(15) . . ?
C9 N2 Cu1 129.7(17) . . ?
C9 N2 C5 118(2) . . ?
C4 N3 H3 117.8 . . ?
C4 N3 C13 124.4(19) . . ?
C13 N3 H3 117.8 . . ?
C1 N4 H4 118.7 . . ?
C1 N4 C14 123(2) . . ?
C14 N4 H4 118.7 . . ?
C8 N5 C11 117(2) . . ?
C10 N6 C3 118(2) . . ?
O2 C1 N4 121(2) . . ?
O2 C1 C6 119(2) . . ?
N4 C1 C6 120(2) . . ?
N1 C2 H2 119.8 . . ?
N1 C2 C10 120(2) . . ?
C10 C2 H2 119.8 . . ?
N6 C3 H3A 119.0 . . ?
N6 C3 C6 122(2) . . ?
C6 C3 H3A 119.0 . . ?
O1 C4 C5 117.0(19) . . ?
N3 C4 O1 120(2) . . ?
N3 C4 C5 123(2) . . ?
N2 C5 C4 114.0(19) . . ?
N2 C5 C8 122(2) . . ?
C8 C5 C4 124(2) . . ?
N1 C6 C1 111.8(18) . . ?
C3 C6 N1 118(2) . . ?
C3 C6 C1 130(2) . . ?
H7A C7 H7B 109.5 . . ?
H7A C7 H7C 109.5 . . ?
H7B C7 H7C 109.5 . . ?
C10 C7 H7A 109.5 . . ?
C10 C7 H7B 109.5 . . ?
C10 C7 H7C 109.5 . . ?
N5 C8 C5 121(2) . . ?
N5 C8 H8 119.7 . . ?
C5 C8 H8 119.7 . . ?
N2 C9 H9 118.8 . . ?
N2 C9 C11 122(2) . . ?
C11 C9 H9 118.8 . . ?
N6 C10 C2 122(2) . . ?
N6 C10 C7 114(2) . . ?
C2 C10 C7 123(2) . . ?
N5 C11 C9 120(2) . . ?
N5 C11 C12 118(2) . . ?
C9 C11 C12 122(2) . . ?
C11 C12 H12A 109.5 . . ?
C11 C12 H12B 109.5 . . ?
C11 C12 H12C 109.5 . . ?
H12A C12 H12B 109.5 . . ?
H12A C12 H12C 109.5 . . ?
H12B C12 H12C 109.5 . . ?
N3 C13 H13A 108.3 . . ?
N3 C13 H13B 108.3 . . ?
N3 C13 C14 116(2) . . ?
H13A C13 H13B 107.4 . . ?
C14 C13 H13A 108.3 . . ?
C14 C13 H13B 108.3 . . ?
N4 C14 C13 116(2) . . ?
N4 C14 H14A 108.4 . . ?
N4 C14 H14B 108.4 . . ?
C13 C14 H14A 108.4 . . ?
C13 C14 H14B 108.4 . . ?
H14A C14 H14B 107.5 . . ?
H1WA O1W H1WB 112.2 . . ?
H2WA O2W H2WB 116.4 . . ?
H3WA O3W H3WB 107.0 . . ?
H4WA O4W H4WB 104.1 . . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
Cu1 O1 C4 N3 177.3(16) . . . . ?
Cu1 O1 C4 C5 -2(2) . . . . ?
Cu1 O2 C1 N4 -177.2(15) 4_676 . . . ?
Cu1 O2 C1 C6 4(2) 4_676 . . . ?
Cu1 N1 C2 C10 -177.5(16) 4_676 . . . ?
Cu1 N1 C6 C1 -2(2) 4_676 . . . ?
Cu1 N1 C6 C3 174.3(16) 4_676 . . . ?
Cu1 N2 C5 C4 6(2) . . . . ?
Cu1 N2 C5 C8 -178.3(18) . . . . ?
Cu1 N2 C9 C11 172.7(18) . . . . ?
O1 C4 C5 N2 -3(3) . . . . ?
O1 C4 C5 C8 -178(2) . . . . ?
O2 C1 C6 N1 -1(3) . . . . ?
O2 C1 C6 C3 -177(2) . . . . ?
O3 W4 O5A W3 -125(2) . . . . ?
O3 W4 O11A W5 -120(3) . . . . ?
O3 W4 O12A W1 126(4) . . . . ?
O3 W4 O16A W2 121(4) . . . . ?
O4 W1 O15A W3 -132(5) 3_566 . . . ?
O4 W2 O14A W5 -144(4) . . . . ?
O4 W2 O16A W4 60(5) . . . . ?
O4 W2 O19 W6 56.2(15) . . . . ?
O5 W4 O3 Cu1 -146(2) . . . . ?
O5A W3 O15A W1 -16(5) . . . . ?
O5A W3 O18A W6 127(5) . . . . ?
O5A W4 O3 Cu1 -132(2) . . . . ?
O5A W4 O11A W5 60(4) . . . . ?
O5A W4 O12A W1 14(4) . . . . ?
O5A W4 O16A W2 -137(5) . . . . ?
O6 W1 O15A W3 -49(5) 3_566 . . . ?
O6 W6 O9 W5 106.4(17) . . . 3_566 ?
O6 W6 O18A W3 -60(5) . . . . ?
O7 W5 O10A W3 125(2) . . . 3_566 ?
O7 W5 O14A W2 -119(3) . . . . ?
O8 W2 O14A W5 118(3) . . . . ?
O8 W2 O16A W4 -120(4) . . . . ?
O8 W2 O19 W6 158.9(14) . . . . ?
O9 W5 O10A W3 21(3) 3_566 . . 3_566 ?
O9 W5 O14A W2 68(5) 3_566 . . . ?
O9 W6 O18A W3 24(4) . . . . ?
O10A W3 O5A W4 -52(3) 3_566 . . . ?
O10A W3 O15A W1 126(5) 3_566 . . . ?
O10A W3 O18A W6 -14(4) 3_566 . . . ?
O10A W5 O14A W2 140(4) . . . . ?
O11 W4 O3 Cu1 32(2) . . . . ?
O11A W4 O3 Cu1 48(2) . . . . ?
O11A W4 O5A W3 55(4) . . . . ?
O11A W4 O12A W1 -126(4) . . . . ?
O11A W4 O16A W2 4(5) . . . . ?
O11A W5 O10A W3 -54(4) . . . 3_566 ?
O11A W5 O14A W2 -2(4) . . . . ?
O12 W4 O3 Cu1 133(2) . . . . ?
O12A W1 O15A W3 16(4) . . . . ?
O12A W4 O3 Cu1 126(2) . . . . ?
O12A W4 O5A W3 -11(3) . . . . ?
O12A W4 O11A W5 134(3) . . . . ?
O12A W4 O16A W2 -61(5) . . . . ?
O13 W3 O5A W4 125(2) . . . . ?
O13 W3 O15A W1 -130(4) . . . . ?
O13 W3 O18A W6 -126(4) . . . . ?
O14 W2 O19 W6 -16(5) . . . . ?
O14A W2 O16A W4 -4(5) . . . . ?
O14A W2 O19 W6 -6(3) . . . . ?
O14A W5 O10A W3 -126(3) . . . 3_566 ?
O15A W3 O5A W4 10(3) . . . . ?
O15A W3 O18A W6 50(5) . . . . ?
O16 W2 O19 W6 -112.0(16) . . . . ?
O16 W4 O3 Cu1 -49(2) . . . . ?
O16A W2 O14A W5 2(4) . . . . ?
O16A W2 O19 W6 -87.7(17) . . . . ?
O16A W4 O3 Cu1 -56(2) . . . . ?
O16A W4 O5A W3 126(3) . . . . ?
O16A W4 O11A W5 -3(3) . . . . ?
O16A W4 O12A W1 -52(5) . . . . ?
O17 W1 O15A W3 128(4) . . . . ?
O18 W6 O9 W5 -63.1(19) . . . 3_566 ?
O18A W3 O5A W4 -126(3) . . . . ?
O18A W3 O15A W1 54(5) . . . . ?
O18A W6 O9 W5 -38.9(18) . . . 3_566 ?
O19 W2 O14A W5 -79(4) . . . . ?
O19 W2 O16A W4 140(5) . . . . ?
O19 W6 O9 W5 31(3) . . . 3_566 ?
O19 W6 O18A W3 -133(4) . . . . ?
O20 W6 O9 W5 -154.9(16) . . . 3_566 ?
O20 W6 O18A W3 126(4) . . . . ?
O21 W1 O15A W3 -32(4) 3_566 . . . ?
O21 W3 O5A W4 -29(2) 3_566 . . . ?
O21 W3 O15A W1 31(4) 3_566 . . . ?
O21 W3 O18A W6 67(4) 3_566 . . . ?
O21 W4 O3 Cu1 171.9(17) 3_566 . . . ?
O21 W4 O5A W3 29(2) 3_566 . . . ?
O21 W4 O11A W5 82(3) 3_566 . . . ?
O21 W4 O12A W1 -30(3) 3_566 . . . ?
O21 W4 O16A W2 -79(4) 3_566 . . . ?
O21 Si1 O22 W2 58.8(17) . . . . ?
O21 Si1 O22 W2 -121.2(17) 3_566 . . . ?
O21 Si1 O22 W4 -179.6(14) . . . . ?
O21 Si1 O22 W4 0.4(14) 3_566 . . . ?
O21 Si1 O22 W5 115.4(17) 3_566 . . . ?
O21 Si1 O22 W5 -64.6(17) . . . . ?
O21 Si1 O23 W1 0.9(16) 3_566 . . . ?
O21 Si1 O23 W1 -179.1(16) . . . . ?
O21 Si1 O23 W6 54(2) . . . 3_566 ?
O21 Si1 O23 W6 -126(2) 3_566 . . 3_566 ?
O21 Si1 O23 O21 179.998(4) . . . 3_566 ?
O21 Si1 O23 O24 -124.2(16) 3_566 . . 3_566 ?
O21 Si1 O23 O24 55.8(16) . . . 3_566 ?
O21 Si1 O24 W3 -177.9(13) . . . . ?
O21 Si1 O24 W3 2.1(13) 3_566 . . . ?
O21 Si1 O24 W5 71.4(17) . . . 3_566 ?
O21 Si1 O24 W5 -108.6(17) 3_566 . . 3_566 ?
O21 Si1 O24 W6 127.1(19) 3_566 . . . ?
O21 Si1 O24 W6 -52.9(19) . . . . ?
O21 Si1 O24 O23 129.1(15) 3_566 . . 3_566 ?
O21 Si1 O24 O23 -50.9(15) . . . 3_566 ?
O22 W2 O14A W5 -38(3) . . . . ?
O22 W2 O16A W4 37(4) . . . . ?
O22 W2 O19 W6 -37.3(15) . . . . ?
O22 W4 O3 Cu1 -11(4) . . . . ?
O22 W4 O5A W3 76(3) . . . . ?
O22 W4 O11A W5 34(3) . . . . ?
O22 W4 O12A W1 -71(4) . . . . ?
O22 W4 O16A W2 -36(4) . . . . ?
O22 W5 O10A W3 -76(3) . . . 3_566 ?
O22 W5 O14A W2 37(3) . . . . ?
O22 Si1 O21 W1 122.0(18) 3_566 . . 3_566 ?
O22 Si1 O21 W1 -58.0(18) . . . 3_566 ?
O22 Si1 O21 W3 70.3(16) . . . 3_566 ?
O22 Si1 O21 W3 -109.7(16) 3_566 . . 3_566 ?
O22 Si1 O21 W4 0.4(13) 3_566 . . 3_566 ?
O22 Si1 O21 W4 -179.6(13) . . . 3_566 ?
O22 Si1 O21 O23 121.1(17) 3_566 . . 3_566 ?
O22 Si1 O21 O23 -58.9(17) . . . 3_566 ?
O22 Si1 O23 W1 -117(2) 3_566 . . . ?
O22 Si1 O23 W1 63(2) . . . . ?
O22 Si1 O23 W6 115.7(19) 3_566 . . 3_566 ?
O22 Si1 O23 W6 -64.3(19) . . . 3_566 ?
O22 Si1 O23 O21 -118.3(15) 3_566 . . 3_566 ?
O22 Si1 O23 O21 61.7(15) . . . 3_566 ?
O22 Si1 O23 O24 117.5(15) 3_566 . . 3_566 ?
O22 Si1 O23 O24 -62.5(15) . . . 3_566 ?
O22 Si1 O24 W3 -66.9(17) . . . . ?
O22 Si1 O24 W3 113.1(17) 3_566 . . . ?
O22 Si1 O24 W5 2.5(14) 3_566 . . 3_566 ?
O22 Si1 O24 W5 -177.5(14) . . . 3_566 ?
O22 Si1 O24 W6 58(2) . . . . ?
O22 Si1 O24 W6 -122(2) 3_566 . . . ?
O22 Si1 O24 O23 60.2(16) . . . 3_566 ?
O22 Si1 O24 O23 -119.8(16) 3_566 . . 3_566 ?
O23 W1 O15A W3 -65(4) . . . . ?
O23 W6 O9 W5 44.3(17) 3_566 . . 3_566 ?
O23 W6 O18A W3 -67(4) 3_566 . . . ?
O23 Si1 O21 W1 0.9(16) 3_566 . . 3_566 ?
O23 Si1 O21 W1 -179.1(16) . . . 3_566 ?
O23 Si1 O21 W3 -50.8(19) . . . 3_566 ?
O23 Si1 O21 W3 129.2(19) 3_566 . . 3_566 ?
O23 Si1 O21 W4 59.3(19) . . . 3_566 ?
O23 Si1 O21 W4 -120.7(19) 3_566 . . 3_566 ?
O23 Si1 O21 O23 180.000(4) . . . 3_566 ?
O23 Si1 O22 W2 -175.8(15) . . . . ?
O23 Si1 O22 W2 4.2(15) 3_566 . . . ?
O23 Si1 O22 W4 125.8(18) 3_566 . . . ?
O23 Si1 O22 W4 -54.2(18) . . . . ?
O23 Si1 O22 W5 -119.3(18) 3_566 . . . ?
O23 Si1 O22 W5 60.7(18) . . . . ?
O23 Si1 O24 W3 52.9(19) . . . . ?
O23 Si1 O24 W3 -127.1(19) 3_566 . . . ?
O23 Si1 O24 W5 -57.7(19) . . . 3_566 ?
O23 Si1 O24 W5 122.3(19) 3_566 . . 3_566 ?
O23 Si1 O24 W6 -2.0(16) 3_566 . . . ?
O23 Si1 O24 W6 178.0(16) . . . . ?
O23 Si1 O24 O23 180.001(11) . . . 3_566 ?
O24 W3 O5A W4 -76(3) . . . . ?
O24 W3 O15A W1 69(4) . . . . ?
O24 W3 O18A W6 31(4) . . . . ?
O24 W5 O10A W3 -28(2) 3_566 . . 3_566 ?
O24 W5 O14A W2 80(4) 3_566 . . . ?
O24 W6 O9 W5 9.4(15) . . . 3_566 ?
O24 W6 O18A W3 -32(4) . . . . ?
O24 Si1 O21 W1 -126.2(19) 3_566 . . 3_566 ?
O24 Si1 O21 W1 53.8(19) . . . 3_566 ?
O24 Si1 O21 W3 2.1(13) 3_566 . . 3_566 ?
O24 Si1 O21 W3 -177.9(13) . . . 3_566 ?
O24 Si1 O21 W4 -67.8(16) . . . 3_566 ?
O24 Si1 O21 W4 112.2(16) 3_566 . . 3_566 ?
O24 Si1 O21 O23 52.9(17) . . . 3_566 ?
O24 Si1 O21 O23 -127.1(17) 3_566 . . 3_566 ?
O24 Si1 O22 W2 -54.0(18) . . . . ?
O24 Si1 O22 W2 126.0(18) 3_566 . . . ?
O24 Si1 O22 W4 67.6(18) . . . . ?
O24 Si1 O22 W4 -112.4(18) 3_566 . . . ?
O24 Si1 O22 W5 -177.5(14) . . . . ?
O24 Si1 O22 W5 2.5(14) 3_566 . . . ?
O24 Si1 O23 W1 -55(2) . . . . ?
O24 Si1 O23 W1 125(2) 3_566 . . . ?
O24 Si1 O23 W6 -1.8(14) 3_566 . . 3_566 ?
O24 Si1 O23 W6 178.2(14) . . . 3_566 ?
O24 Si1 O23 O21 124.2(16) 3_566 . . 3_566 ?
O24 Si1 O23 O21 -55.8(16) . . . 3_566 ?
O24 Si1 O23 O24 180.001(10) . . . 3_566 ?
N1 C2 C10 N6 4(4) . . . . ?
N1 C2 C10 C7 -173(2) . . . . ?
N2 C5 C8 N5 6(4) . . . . ?
N2 C9 C11 N5 3(4) . . . . ?
N2 C9 C11 C12 -179(2) . . . . ?
N3 C4 C5 N2 178(2) . . . . ?
N3 C4 C5 C8 2(4) . . . . ?
N3 C13 C14 N4 -154(2) . . . . ?
N4 C1 C6 N1 -179.8(18) . . . . ?
N4 C1 C6 C3 4(4) . . . . ?
N6 C3 C6 N1 4(3) . . . . ?
N6 C3 C6 C1 180(2) . . . . ?
C1 N4 C14 C13 -142(2) . . . . ?
C2 N1 C6 C1 179.2(19) . . . . ?
C2 N1 C6 C3 -4(3) . . . . ?
C3 N6 C10 C2 -4(3) . . . . ?
C3 N6 C10 C7 173(2) . . . . ?
C4 N3 C13 C14 -172(2) . . . . ?
C4 C5 C8 N5 -178(2) . . . . ?
C5 N2 C9 C11 -2(4) . . . . ?
C6 N1 C2 C10 1(3) . . . . ?
C8 N5 C11 C9 0(3) . . . . ?
C8 N5 C11 C12 -178(2) . . . . ?
C9 N2 C5 C4 -179(2) . . . . ?
C9 N2 C5 C8 -3(3) . . . . ?
C10 N6 C3 C6 0(3) . . . . ?
C11 N5 C8 C5 -5(3) . . . . ?
C13 N3 C4 O1 -1(3) . . . . ?
C13 N3 C4 C5 179(2) . . . . ?
C14 N4 C1 O2 1(3) . . . . ?
C14 N4 C1 C6 180(2) . . . . ?

_olex2_submission_special_instructions 'No special instructions were received'
